Synthesis, Structural, and Adsorption Properties and Thermal Stability of Nanohydroxyapatite/Polysaccharide Composites
© The Author(s). 2017
Received: 30 December 2016
Accepted: 9 February 2017
Published: 27 February 2017
A series of composites based on nanohydroxyapatite (nHAp) and natural polysaccharides (PS) (nHAp/agar, nHAp/chitosan, nHAp/pectin FB300, nHAp/pectin APA103, nHAp/sodium alginate) was synthesized by liquid-phase two-step method and characterized using nitrogen adsorption–desorption, DSC, TG, FTIR spectroscopy, and SEM. The analysis of nitrogen adsorption–desorption data shows that composites with a nHAp: PS ratio of 4:1 exhibit a sufficiently high specific surface area from 49 to 82 m2/g. The incremental pore size distributions indicate mainly mesoporosity. The composites with the component ratio 1:1 preferably form a film-like structure, and the value of S BET varies from 0.3 to 43 m2/g depending on the nature of a polysaccharide. Adsorption of Sr(II) on the composites from the aqueous solutions has been studied. The thermal properties of polysaccharides alone and in nHAp/PS show the influence of nHAp, since there is a shift of characteristic DSC and DTG peaks. FTIR spectroscopy data confirm the presence of functional groups typical for nHAp as well as polysaccharides in composites. Structure and morphological characteristics of the composites are strongly dependent on the ratio of components, since nHAp/PS at 4:1 have relatively large S BET values and a good ability to adsorb metal ions. The comparison of the adsorption capacity with respect to Sr(II) of nHAp, polysaccharides, and composites shows that it of the latter is higher than that of nHAp (per 1 m2 of surface).
KeywordsNanohydroxyapatite High- and low-esterified pectins Agar Sodium alginate Chitosan Composites Sr(II) adsorption
In recent years, intense researches are carried out to prepare bio-hydroxyapatite composites with desired biological, physical, and mechanical properties. Hydroxyapatite and its composites are of interest due to applications in medicine. The physicochemical properties and biocompatibility make them a very attractive object for investigations both in vivo and in vitro [1–19].
Modification of hydroxyapatite (HAp) with such natural polysaccharides as chitosan [3–6], sodium alginate [7–13], agar [14, 15] and pectins [16–19], or embedding HAp nanoparticles into a polymer matrix as a filler allows one to control the morphological, structural, and mechanical properties of composites to enhance the functional use. The composites based on chitosan with HAp or alginate are mainly used to treat bone implants [3–8, 11–14, 16–18] or to use as drugs carriers [9, 10, 15].
Analysis of the literature shows that the synthesis of HAp/PS composites, their use, and control of the properties are far from exhausted ones. The use of HAp/PS composites as adsorbents could be promising since the components alone show a high adsorption capacity with respect to heavy metal cations [20–34]. Creation of composites allows one to control the structure of the materials to improve the morphology and to enhance the adsorption properties. It is known that natural polysaccharides are good sorbents of some kinds of dyes [29–31, 35] and heavy metal ions [23–33] because of specific interactions of the amino and hydroxyl groups with adsorbates . The amino groups of polysaccharides can be cationized that allows the effective adsorption of ionic dyes . However, the use of some polysaccharides in their native form is difficult since the viscosity of the solutions is high even at a low concentration because of tendency to gelling. Therefore, composites with PS can be more appropriate for the adsorption applications due to diminution of the mentioned negative effects [39–41]. Immobilization of macromolecules on a HAp surface allows an increase in sorption activity of the composites compared to the components alone.
The objective of this work was the synthesis of nHAp/polysaccharide composites and the study of the structural and morphological characteristics, the thermal behavior, and sorption capacity with respect to Sr(II).
calcium hydroxide (Aldrich) and phosphoric acid (POCh, Gliwice) were used as 1 M aqueous solutions of 0.18 and 0.3 L, respectively. The H3PO4 solution was dropped into the Ca(OH)2 suspension placed in a flask for 15 min. While dropping the reaction, mixture was stirred vigorously and then dried in a dryer at 80 °C for 24 h. A white sediment with crystalline hydroxyapatite was obtained. Then the sediment was washed with redistilled water till the constant value of redistilled water conductivity was achieved. The average crystallite size determined from XRD patterns using Scherrer’s equation applied to a peak at 2θ = 25.9 was 26 nm. The degree of crystallinity  was 22%.
The second stage was the synthesis of nHAp/polysaccharide composites using chitosan (deacetylation degree 82%, “Bioprogress” CJSC, Moscow, Russia), high-etherified apple pectin APA 103 at the degree of etherification (DE) of 66–68% and low-etherified apple pectin APA 300 FB with galacturonic acid with free carboxyl groups 64–69% (Andre Pectin, China), and sodium alginate (SA) at a mass fraction of the basic substance of 99.0% (China) as received. nHAp composites were prepared by mixing of the nHAp suspension and PS solution. Additionally, the polysaccharide solution (2 wt.%) and nHAp suspension (4 wt.%) sonicated for 3 min were prepared using distilled water, mixed at the nHAp/PS ratio of 1:1 and 4:1, and stirred for 30 min. Then the nHAp/PS suspensions were dried at 40 °C in air.
The hydroxyl groups are the main functional groups of PS, which can be esterified or oxidized. The carboxyl groups of uronic acid can be esterified, and the amino groups of amino sugars can be acylated. Modified PS are capable to create strong complexes with metal ions, as well as with polar low-molecular weight organics.
The formation of composites occurs due to strong interactions of the phosphate and hydroxyl groups of nHAp with the COO−, OH, and other polar groups in PS . The polysaccharide molecules also tend to form the hydrogen bonds with each other resulting in gelation of their aqueous solutions upon heating at certain temperatures. The calcium phosphate ions can be trapped in the PS chains. The cross-linking reactions may occur in the composites. Therefore, nHAp nanoparticles could be well distributed in the PS network and remained in stable state for a long period.
Fourier Transform Infrared (FTIR) Spectroscopy
FTIR spectra of powdered samples (grinded with dry KBr at the mass ratio 1:9) over the 4000–400 cm−1 range were recorded using a ThermoNicolet FTIR spectrometer with a diffuse reflectance mode.
Scanning electron microscopy (SEM)
The surface morphology of composites was analyzed using field emission scanning electron microscopy employing a QuantaTM 3D FEG (FEI, USA) apparatus operating at the voltage of 30 kV.
Specific surface areas and pore volumes were determined from low-temperature nitrogen adsorption isotherms using a Micromeritics ASAP 2020 or 2405N adsorption analyzer. Before measurements, the samples were outgassed at 80 °C for 12 h. The nitrogen desorption data were used to compute the pore size distributions (PSD, differential f V ~ dV p/dR and f S ~ dS/dR) using a self-consistent regularization (SCR) procedure under non-negativity condition (f V ≥ 0 at any pore radius R) at a fixed regularization parameter α = 0.01 using a model of voids (V) between spherical nonporous nanoparticles packed in random aggregates (V/SCR model) . The differential PSD with respect to the pore volume f V ~ dV/dR, ∫ f VdR ~ V p were re-calculated to incremental PSD (IPSD) at ΦV(R i ) = (f V(R i+1) + f V(R i ))(R i+1 − R i )/2 at ∑ΦV(R i ) = V p. The f V and f S functions were also used to calculate contributions of micropores (V micro and S micro at 0.35 nm < R < 1 nm), mesopores (V meso and S meso at 1 nm < R < 25 nm), and macropores (V macro and S macro at 25 nm < R < 100 nm).
Thermal analysis was carried out using a STA 449 Jupiter F1 (Netzsch, Germany) apparatus, sample mass ~16 mg placed into a corundum crucible, air flow of 50 mL min−1, a heating rate of 10 °C min−1, temperature range of 30–950 °C, and S TG-DSC sensor thermocouple type. Empty corundum crucible was used as a reference. The gaseous products emitted during decomposition of the materials were analyzed by using a FTIR Brucker (Germany) spectrometer and QMS 403D Aëolos (Germany) coupling on-line to STA instrument. The QMS data were gathered in the range from 10 to 200 a.m.u. The FTIR spectra were recorded in the range of 4000–600 cm−1 with 16 scans per spectrum at a resolution of 4 cm−1.
Adsorption of Sr(II)
The adsorption of Sr(II) ions vs. pH at the composite/electrolyte solution interface was determined by the means of the radioisotope method. The initial concentration of Sr(II) ions was 10−4 M. NaCl (0.001 mol/dm3) was used as a background electrolyte, and pH was changed from 3 to 10. The adsorption measurements were complemented by the potentiometric titration of the composites in the suspensions and the electrophoresis measurements. The adsorption measurements were performed in a thermostated Teflon vessel at 25 °C. To eliminate CO2, all the potentiometric measurements and adsorption experiments were carried out under the nitrogen atmosphere. The pH values were measured using a set of glass REF 451 and calomel pHG201-8 electrodes with Radiometer assembly. Radioactivity of the solutions before and after adsorption was measured using a LS 5000 TD Beckmann liquid scintillation counter. Because 90Sr decays to the radioactive 90Y, the measurements were carried out in two channels in order to calculate radioactivity of 90Sr.
Results and Discussion
Textural characteristics of initial nHAp and nHAp/PS nanocomposites
S BET (m2/g)
S micro (m2/g)
S meso (m2/g)
S macro (m2/g)
V p (cm3/g)
V micro (cm3/g)
V meso (cm3/g)
V macro (cm3/g)
R p,V (nm)
The hysteresis loop shape indicates dominant contribution of mesopores (filled by adsorbed nitrogen during the measurements). It should be noted that in the case of highly disperse materials, only a certain part of pores can be filled by nitrogen because large macropores remain empty, i.e., V p < V em = 1/ρ b − 1/ρ 0, where ρ b and ρ 0 are bulk and true densities of the materials.
A film-like, near-monolithic structure is formed in nHAp/PS at the ratio of 1:1 (Fig. 3b, d) as evidenced by low values of the specific surface area. However, some porosity of the composites remains. At the component ratio of 4:1, the structure of composites is more porous and can be described as multimodal aggregates of nHAp/PS with sizes over a wide range of 20–250 nm (Fig. 3c, e). Similar structure of aggregates of primary particles inherent to initial nHAp (Fig. 3a), and it remains for composites nHAp/pectins and nHAp/SA (Fig. 4). Thus, a relatively high value of S BET and porous structure of these composites (Table 1, Figs. 1, 2, 3, and 4) indicate the prospects for their use as better adsorbents than those at 50 wt.% of PS.
Fourier Transform Infrared Spectroscopy (FTIR)
The presence of (CO3)2 groups is confirmed by bands at 1414 cm−1, which are assigned to stretching mode of the (CO3)2 groups [46, 51–53], and at 1465 cm−1, which can be attributed to the stretching modes of the (CO3)2 groups in A-type of carbonated apatite [46, 54, 55].
OH groups and adsorbed water molecules, presented in the hydroxyapatite sample, give peaks at 875 cm−1 (hydrogen phosphate groups) and 2856–3656 cm−1 with a maximum at 3400 cm−1.
All characteristic bands of hydroxyapatite remain in the IR spectra of the nHAp/PS composites (Fig. 5), but their intensity decreases with decreasing content of hydroxyapatite. The appearance the bands at 2927 and 2851 cm−1 is due to C–H asymmetric and symmetric stretching vibrations in the aliphatic CH2 groups of PS. Especially noticeable increase in intensity of broad band with a maximum at 3445 cm−1 is due to the OH groups in PS forming the hydrogen bonds with each other or adsorbed water molecules. Additionally, the N–H bonds in the amino groups of chitosan give the bands at ~3350 cm−1. Similar features of the IR spectra of nHAp/pectin are shown in Fig. 5b. Pectin molecules include few hundred linked galacturonic acid residues forming a long molecular chain with polygalacturonic acid, wherein a fraction of galacturonic acid subunits is methoxylated. The pectin molecules contain a large amount of carboxyl (free and esterified), hydroxyl, methoxyl, and acetyl groups. The bands at 2926 and 2852 cm−1 of the C–H stretching vibrations and a broad band with a maximum at 3445 cm−1 increase with increasing content of pectins. The IR spectra of pectins are characterized by bands at 1750–1700 cm−1 related to the stretching vibrations of the carbonyl, ester, and carboxyl groups. The IR spectra of nHAp/sodium alginate (Fig. 5c) show similar bands of the hydroxyl, ether, and carboxylic groups, as well as the O–H and C–H stretching vibrations of alginate. Bands at 1633 and 1460 cm−1 can be attributed to the asymmetric and symmetric stretching vibrations of carboxylate salt ions. These bands can be used to characterize structures of alginate, its derivatives, and ingredients.
TG and DTG curves of pectin FB300 characterize decomposition of the polymer chain in the first stage from 203 to 337 °C with maxima at 226.3 and 302.9 °C (Fig. 6c, Additional file 1: Table S1). For composites, three degradation peaks at 204.1, 250.1, and 316.2 °C are observed (Fig. 6d, Additional file 1: Table S1). The temperature range of PS degradation becomes wider compared with the pectin alone. The amount of physically adsorbed water is less in the composite than the pectin alone. Decomposition of pectin APA103 begins at lower temperatures than that of pectin FB300. The peak of pectin degradation in composites is slightly shifted toward lower temperatures.
Thermal effects upon degradation of polysaccharides can be estimated from the DSC data (Fig. 7). A weak endothermic peak between 50 and 150 °C with a maximum of ca. One hundred degree Celcius can be attributed to desorption of intact water. Thermodegradation of polysaccharides is usually accompanied by an exothermic effect. Typical DSC curves (Fig. 7) show three main peaks upon thermal analysis of sodium alginate and chitosan, and two peaks for agar. It is noteworthy that the intensive peaks distinguishable for initial (bulk) sodium alginate on DSC curve at 583.6 °C (Fig.7a) and DTG curve at 580.7 °C (Fig.6a) strongly changed for composite nHAp/SA: DSC peak disappears (Fig.7b), and DTG peak has much smaller intensity and shifted to temperature 672.7 °C (Fig.6b). The similar regularities are also observed for other composites HAp/PS: high-temperature peaks distinguishable on the DSC curves for bulk agar at 460.7 °C (Fig.7a), for bulk pectin FB300 at 746.7 and 586.6 °C, for bulk pectin APA103 at 593.3 °C (Fig.7c) are not observed on DSC curves for the corresponding composites nHAp/PS (Fig.7b, d). In the case of chitosan, all temperature peaks on DCS curve of bulk polysaccharide appear in DCS curve for the nHAp/chitosan composite but shifted to lower temperatures (Fig.7a, b). On DTG curves of composites agar/MS and pectin FB300/PS, the shift toward lower temperatures is observed for high-temperature peaks compared to the DTG curves for the initial polysaccharides: DTG peak for bulk agar at 457.5 °C shifted to 381.2 °C; peak on the DTG curve for pectin FB300 at 742.7 °C has disappeared on DTG curve for the composite; and the peak at 581.3 ° C shifted to 504.4 ° C. DTG peaks shifted slightly for nHAp/APA103 composites compared with initial pectin (Fig. 6c, d). Such peculiarities show that a strong interaction PS with nHAp results in a significant change in the thermal properties of PS. The multiple exothermic peaks of pectin degradation are observed at T > 150 °C, wherein for pectin FB300, it is not clear separation of peaks indicating the complexity and manifold of processes of degradation, while for pectin APA103 main peak is at 436 ° C.
Adsorption of Sr(II)
The pH dependences of the Sr2+ adsorption vary for composites with different PS. For nHAp/agar and nHAp/chitosan, it is also observed a monotonic pH dependence of the Sr2+ adsorption, but the adsorption is higher than for the initial nHAp. The high values of the adsorption and a small remnant of the solution is achieved at a pH greater than 8 (Fig. 9a). For composites containing pectins, higher values of the adsorption are observed in the acidic pH range. In the case of nHAp/pectin FB300 composite, the Sr2+ adsorption reaches 0.25 μmol/m2 at pH 6.5 (Fig. 9b).
For nHAp/PS, two mechanisms of the adsorption can be realized due to Sr(II) interactions with nHAp or polysaccharides. The adsorption of metal ions on polysaccharides occurs with participation of carboxyl groups of pectin, agar and sodium alginate, and amino groups in chitosan, which are capable of strong electrostatic interactions with metal ions [24–26, 35–37]. Therefore, all the composites studied show the adsorption capacity with respect to Sr(II) higher than the initial nHAp.
Thus, nHAp/PS with different polysaccharides and different nHAp:PS ratios 4:1 and 1:1 synthesized by two-step process demonstrate certain decrease in the textural characteristics with increasing content of PS due to filling of inter-particle voids by polymers. However, the composites that have the HAP:PS ratio of 4:1 show relatively developed SBET from 49 m2/g for nHAp/pectin FB300 to 82 m2/g for nHAp/SA. Mainly mesoporosity is the characteristic for the composites, since contribution of micro and macro pores is negligible. At the nHAp:PS ratio 1:1, a film-like structure was formed. The specific surface area and porosity largely depend on the nature of the polysaccharide, and maximal SBET value of 43 m2/g is for nHAp/agar. The thermal properties of the composites show a certain influence of nHAp on polysaccharide degradation. However, composites have sufficient thermal stability. In the composites, the polysaccharide degradation occurs at temperatures above 200 °C. It was found out that for nHAp/PS composites at the component ratio 4:1, the adsorption capacity with respect to Sr2+ ions is higher than for the initial nHAp. This makes these composite promising for the use as adsorbents for metal cations from aqueous media.
The authors are grateful to European Community, Seventh Framework Programme (FP7/2007–2013), Marie Curie International Research Staff Exchange Scheme (IRSES grant No. 612484) for financial support of this work. The research was partly carried out with the equipment purchased thanks to the financial support of the European Regional Development Fund in the framework of the Polish Innovation Economy Operational Program (contract no. POIG.02.01.00-06-024/09 Center of Functional Nanomaterials).
ES carried out the synthesis of nHAp and characterization of nanocomposites by SEM method, participated in characterization of nanocomposites by FTIR method and adsorption of Sr2+. OG carried out the synthesis of nHAp/PS nanocomposites. DS participated in DSC and TG studies. KG carried out the nitrogen adsorption–desorption measurements. OG and VMG analyzed the data and drafted the manuscript. WJ and VMG revised the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Venkatesan J, Kim SJ (2014) Nano-hydroxyapatite composite biomaterials for bone tissue engineering—a review. J Biomed Nanotechnol 10(10):3124–40. doi:https://doi.org/10.1166/jbn.2014.1893 View ArticleGoogle Scholar
- Skwarek E, Janusz W, Gun’ko VM, Pakhlov EM, Zarko VI, Gdula K (2016) Characteristics of surface and electrochemical properties of composites with fumed metal oxides and hydroxyapatite. Adsorption 22:725–734. doi:https://doi.org/10.1007/s10450-016-9770-4 View ArticleGoogle Scholar
- Pangon A, Saesoo S, Saengkrit N, Ruktanonchai U, Intasanta V (2016) Hydroxyapatite-hybridized chitosan/chitin whisker bionanocomposite fibers for bone tissue engineering applications. Carbohydr Polym 144:419–427View ArticleGoogle Scholar
- Lowe B, Venkatesan J, Anil S, Shim MS, Kim SK (2016) Preparation and characterization of chitosan-natural nanohydroxyapatite-fucoidan nanocomposites for bone tissue engineering. Int J Biol Macromol 93:1479–1487View ArticleGoogle Scholar
- Rogina A, Ivanković M, Ivanković H (2013) Preparation and characterization of nano-hydroxyapatite within chitosan matrix. Mater Sci Eng C 33:4539–4544View ArticleGoogle Scholar
- Tsiourvas D, Sapalidis A, Papadopoulos T (2016) Hydroxyapatite/chitosan-based porous three-dimensional scaffolds with complex geometries. Mater Today Com 7:59–66View ArticleGoogle Scholar
- Son KD, Yang DJ, Kim MS, Kang IK, Kim SY, Kim YJ (2012) Effect of alginate as polymer matrix on the characteristics of hydroxyapatite nanoparticles. Mater Chem Phys 132:1041–1047View ArticleGoogle Scholar
- Venkatesan J, Bhatnagar I, Manivasagan P, Kang KH, Kim SK (2015) Alginate composites for bone tissue engineering: a review. Int J Biol Macromol 72:269–281View ArticleGoogle Scholar
- Ilie A, Ghiţulică C, Andronescu E, Cucuruz A, Ficai A (2016) New composite materials based on alginate and hydroxyapatite as potential carriers for ascorbic acid. Int J Pharm 510:501–507View ArticleGoogle Scholar
- Yan J, Miao Y, Tan H, Zhou T, Ling Z, Chen Y, Xing X, Hu X (2016) Injectable alginate/hydroxyapatite gel scaffold combined with gelatin microspheres for drug delivery and bone tissue engineering. Mater Sci Eng C 63:274–284View ArticleGoogle Scholar
- Rajkumar M, Meenakshisundaram N, Rajendran V (2011) Development of nanocomposites based on hydroxyapatite/sodium alginate: synthesis and characterization. Mater Charact 62:469–479View ArticleGoogle Scholar
- Kamalaldin NA, Yahya BH, Nurazreena A (2016) Cell evaluation on alginate/hydroxyapatite block for biomedical application. Procedia Chemistry 19:297–303View ArticleGoogle Scholar
- Munarina F, Petrinia P, Gentilinia R, Pillaib RS, Dirèb S, Tanzia MC, Sglavoba VM (2015) Laboratorio micro- and nano-hydroxyapatite as active reinforcement for soft biocomposites. Int J Biol Macromolec 72:199–209View ArticleGoogle Scholar
- Hu J, Zhu Y, Tong H, Shen X, Chen L, Ranba J (2016) A detailed study of homogeneous agarose/hydroxyapatite nanocomposites for load-bearing bone tissue. Int J Biol Macromolec 82:134–143View ArticleGoogle Scholar
- Kolanthai E, Ganesan K, Epple M, Kalkura SN (2016) Synthesis of nanosized hydroxyapatite/agarose powders for bonefiller and drug delivery application. Mater Today Com 8:31–40View ArticleGoogle Scholar
- Munarin F, Petrini P, Gentilini R, Pillai RS, Dirè S, Tanzi MC, Sglavo VM (2015) Micro- and nano-hydroxyapatite as active reinforcement for soft biocomposites. Int J Biol Macromolec 72:199–209View ArticleGoogle Scholar
- Li J, Sun H, Sun D, Yao Y, Yao F, Yao K (2011) Biomimetic multicomponent polysaccharide/nano-hydroxyapatite composites for bone tissue engineering. Carbohydr Polym 85:885–894View ArticleGoogle Scholar
- Li J, Zhu D, Yin J, Liu Y, Yao F, Yao K (2010) Formation of nano-hydroxyapatite crystal in situ in chitosan–pectin polyelectrolyte complex network. Mater Sci Eng C 30:795–803View ArticleGoogle Scholar
- Munarin F, Petrini P, Barcellona G, Roversi T, Piazza L, Visai L, Tanzi MC (2014) Reactive hydroxyapatite fillers for pectin biocomposites. Mater Sci Eng C 45:154–161View ArticleGoogle Scholar
- Janusz W, Skwarek E (2016) Study of sorption processes of strontium on the synthetic hydroxyapatite. Adsorption. 22(4). DOI: https://doi.org/10.1007/s10450-016-9761-5.
- Skwarek E, Janusz W (2016) Adsorption of Cd(II) ions at the hydroxyapatite/electrolyte solution interface. Separ Sci Technol 51(1):11–21View ArticleGoogle Scholar
- Skwarek E (2015) Adsorption of Cs + at the hydroxyapatite/aqueous electrolyte interface.II. Adsor Sci Techn 33(6-8):575–580View ArticleGoogle Scholar
- Abdel-Halim ES, Al-Deyab SS (2011) Removal of heavy metals from their aqueous solutions through adsorption onto natural polymers. Carbohydr Polym 84(1):454–458View ArticleGoogle Scholar
- Kartel MT, Kupchik LA, Veisov BK (1999) Evaluation of pectin binding of heavy metal ions in aqueous solutions. Chemosphere 38(11):2591–2596View ArticleGoogle Scholar
- Dronnet VM, Renard CMGC, Axelos MAV, Thibault JF (1996) Characterisation and selectivity of divalent metal ions binding by citrus and sugar-beet pectins. Carbohydr Polym 30:253–263View ArticleGoogle Scholar
- Hong HJ, Ryu J, Park IS, Ryu T, Chung KS, Kim BG (2016) Investigation of the strontium (Sr(II)) adsorption of an alginate microsphere as a low-cost adsorbent for removal and recovery from seawater. J Environ Manage 165:263–270. doi:https://doi.org/10.1016/j.jenvman.2015.09.040 View ArticleGoogle Scholar
- Li FT, Yang H, Zhao Y, Xu R (2007) Novel modified pectin for heavy metal adsorption. Chin Chem Lett 18:325–328View ArticleGoogle Scholar
- Mata YN, Blázquez ML, Ballester A, González F, Munoz JA (2009) Sugar-beet pulp pectin gels as biosorbent for heavy metals: preparation and determination of biosorption and desorption characteristics. Chem Eng J 150:289–301View ArticleGoogle Scholar
- Ngah WSW, Teonga LC, Hanafiaha MAKM (2011) Adsorption of dyes and heavy metal ions by chitosan composites: a review. Carbohydr Polym 83:1446–1456View ArticleGoogle Scholar
- Kumar MNVR (2000) A review of chitin and chitosan applications. React Funct Polym 46:1–27View ArticleGoogle Scholar
- Liu B, Wang D, Yu G, Meng X (2013) Adsorption of heavy metal ions, dyes and proteins by chitosan composites and derivatives—a review. JOUC 12(3):500–508Google Scholar
- Ren H, Gao Z, Wu D, Jiang J, Sun Y, Luo C (2016) Efficient Pb(II) removal using sodium alginate–carboxymethylcellulose gel beads: preparation, characterization, and adsorption mechanism. Carbohydr Polym 137:402–409View ArticleGoogle Scholar
- Khozhaenko E, Kovalev V, Podkorytova E, Khotimchenko M (2016) Removal of the metal ions from aqueous solutions by nanoscaled low molecular pectin isolated from seagrass Phyllospadix iwatensis. Sci Total Environ 565:913–921View ArticleGoogle Scholar
- Lakouraj MM, Mojerlou F, Zare EN (2014) Nanogel and superparamagnetic nanocomposite based on sodium alginate for sorption of heavy metal ions. Carbohydr Polym 106:34–41View ArticleGoogle Scholar
- Reddad Z, Gerente C, Andres Y, Le Cloirec P (2002) Adsorption of several metal ions onto a low-cost biosorbent: kinetic and equilibrium studies. Environ Sci Technol 36(9):2067–73View ArticleGoogle Scholar
- Crini G (2006) Non-conventional low-cost adsorbents for dye removal: a review. Bioresource Technol 97:1061–1085View ArticleGoogle Scholar
- Wu FC, Tseng RL, Juang RS (2001) Kinetic modeling of liquid-phase adsorption of reactive dyes and metal ions on chitosan. Water Res 35:613–618View ArticleGoogle Scholar
- Kumar V, Kiran K (2000) The effect of retail environment on retailer performance. J Bus Res 49:167–181View ArticleGoogle Scholar
- Budnyak TM, Yanovska ES, Kołodyn´ska D, Sternik D, Pylypchuk IV, Ischenko MV, Tertykh VA (2016) Preparation and properties of organomineral adsorbent obtained by sol–gel technology. J Therm Anal Calorim 125:1335–1351. doi:https://doi.org/10.1007/s10973-016-5581-9 View ArticleGoogle Scholar
- Asgari S, Jahanshahi M, Rahimpour A (2014) Cost-effective nanoporous agar–agar polymer/nickel powder composite particle for effective bio-products adsorption by expanded bed chromatography. J Chromatogr A 1361:191–202View ArticleGoogle Scholar
- Sharma G, Pathania D, Naushad M (2014) Preparation, characterization and antimicrobial activity of biopolymer based nanocomposite ion exchanger pectin zirconium(IV) selenotungstophosphate: application for removal of toxic metals. J Ind Eng Chem 20:4482–4490View ArticleGoogle Scholar
- Landi E, Tampieri A, Celotti G, Sprio S (2000) Desiccation behavior and mechanisms of synthetic hydroxyapatites. J Eur Ceram Soc 20:2377–2387View ArticleGoogle Scholar
- Gun’ko VM (2014) Composite materials: textural characteristics. Applied Surface Sci 307:444–454. doi:https://doi.org/10.1016/j.apsusc.2014.04.055 View ArticleGoogle Scholar
- Sing KSW, Everett DH, Haul RAW, Moscou L, Pieroti RA, Rouquerol J, Siemieniewska T (1985) Reporting phisorption data for gas/solid systems. Pure Appl Chem 57Google Scholar
- Thommes M, Kaneko K, Neimark AV, Olivier JP, Rodriguez-Reinoso F, Rouquerol J, Sing KSW (2015) Pure Appl. Chem.; aop; IUPAC Technical Report; Physisorption of gases, with special reference to the evaluation of surface area and pore size distribution (IUPAC Technical Report). doi:https://doi.org/10.1515/pac-2014-1117.
- Koutsopoulos S (2002) Synthesis and characterization of hydroxyapatite crystals: a review study on the analytical methods. J Biomed Mater Res 62(4):600–12. doi:https://doi.org/10.1002/jbm.10280 View ArticleGoogle Scholar
- Fowler BO (1974) Infrared studies of apatites. I. Vibrational assignments for calcium, strontium, and barium hydroxyapatites utilizing isotopic substitution. Inorg Chem 13:194–207View ArticleGoogle Scholar
- Klee WE, Engel G (1970) Infrared spectra of the phosphate ions in various apatites. J Inorg Nucl Chem 32:1837–1843View ArticleGoogle Scholar
- Rey C, Shimizu M, Collins B, Glimcher MJ (1991) Resolution-enhanced Fourier-transform infrared spectroscopy study of the environment of phosphate ion in the early deposits of a solid phase of calcium phosphate in bone and enamel and their evolution with age: 2. Investigations in the 3PO4 domain. Calcif Tissue Int 49:383–388View ArticleGoogle Scholar
- Gadaleta SJ, Paschalis EP, Camacho NP, Betts F, Mendelhson R, Boskey AL (1995) Fourier transform infrared spectroscopy of synthetic and biological apatites. In: Amjad Z (ed) Mineral scale formation and inhibition. Plenum Press, New York, pp 283–294View ArticleGoogle Scholar
- Baddiel CB, Berry EE (1966) Spectra-structure correlations in hydroxyapatite and fluorapatite. Spectrochim Acta A 22:1407–1416View ArticleGoogle Scholar
- Arends J, Christoffersen J, Christoffersen MR, Eckert H, Fowler BO, Heughebaert JC, Nancollas GH, Yesinowski JP, Zawacki SJ (1987) A calcium hydroxyapatite precipitated from an aqueous solution; an international multimethod analysis. J Crystal Growth 84:512–532View ArticleGoogle Scholar
- Nelson DGA, Featherstone JDB (1982) Preparation, analysis, and characterization of carbonated apatites. Calcif Tissue Int 34(Suppl 2):69–81Google Scholar
- Meyer JL, Fowler BO (1982) Lattice defects in nonstoichiometric calcium hydroxylapatites. A chemical approach. Inorg Chem 21:3029–3035View ArticleGoogle Scholar
- Montel G (1968) Physical chemistry of phosphate with the apatite structure Bull Soc Chim France Spec No:1693–1700.Google Scholar
- Skwarek E, Janusz W, Sternik D (2014) Adsorption of citrate ions on hydroxyapatite synthetized by various methods. J Radioanal Nucl Chem 299:2027–2036View ArticleGoogle Scholar
- Yariv S (2004) The role of charcoal on DTA curves of organo-clay complexes: an overview. Appl Clay Sci 24:225–36View ArticleGoogle Scholar
- He H, Frost RL, Bostrom T, Yuan P, Duong L, Yang D, Xi Y, Kloprogge JT (2006) Changes in the morphology of organoclays with HDTMA+ surfactant loading. Appl Clay Sci 31:262–271View ArticleGoogle Scholar
- Majdan M, Pikus S, Rzączyńska Z, Iwan M, Maryuk O, Kwiatkowski R, Skrzypek H (2006) Characteristics of chabazite modified by hexadecyltrimethylammonium bromide and of its affinity toward chromates. J Mol Struct 791:53–60View ArticleGoogle Scholar
- Estrela dos Santos J, Dockal ER, Cavalheiro ÉTG (2005) Thermal behavior of Schiff bases from chitosan. J Therm Anal Calorim 79:243–248View ArticleGoogle Scholar
- López FA, Mercĕ ALR, Alguacil FJ, López-Delgado A (2008) A kinetic study on the thermal behaviour of chitosan. J Therm Anal Calorim 91(2):633–639View ArticleGoogle Scholar
- Ross AB, Hall C, Anastasakis K, Westwood A, Jones JM, Crewe RJ (2011) Influence of cation on the pyrolysis and oxidation of alginates. J Anal Appl Pyrol 91:344–351View ArticleGoogle Scholar
- Soares JP, Santos JE, Chierice GO, Cavalheiro ETG (2004) Thermal behavior of alginic acid and its sodium salt. Eclet Quim 29(2):53–56View ArticleGoogle Scholar
- Smicˇiklas I, Dimovic S, Plec´as I, Mitric M (2006) Removal of Co2+ from aqueous solutions by hydroxyapatite. Water Res 40:2267–2274View ArticleGoogle Scholar